photodegradation of polypropylene with sorbitol-based nucleating
Post on 03-Jan-2017
Embed Size (px)
Photodegradation of Polypropylene with sorbitol-based nucleating agent
ROMAN ERMK, JANA NAVRTILOV, LEO VAEKDepartment of Polymer Engineering
Tomas Bata University in Zln, Faculty of Technologynm. T. G. Masaryka 275, 762 72 Zln
CZECH REPUBLICcermak@ft.utb.cz http://www.ft.utb.cz
Abstract: - The paper deals with the effects of nucleation on photodegradation of isotactic polypropylene. The starting polymer was modified by a specific -nucleating/clarifying agent Millad 3988 based on 1,3;2,4-bis(3,4-dimethylbenzylidene) sorbitol. Several concentrations were applied. Samples prepared by compression moulding were then exposed to UV-irradiation. Infrared spectroscopy showed that the degradation kinetics is similar for all the samples. Melting and crystallization behaviour of irradiated samples was followed using a differential scanning calorimetry. In all cases UV-irradiation led to decrease of melting/crystallization temperature as a result of polymer degradation. The surface cracking was observed using polarized light microscopy. The network of the surface cracking was significantly different for neat and nucleated samples.
Key-Words: - polypropylene, nucleating agent, sorbitol, photodegradation, polymorphism
1 IntroductionMacroscopic behaviour of polymeric materials within their lifecycle is generally determined by their chemical nature. However, processability, applicability and durability of plastics can be essentially influenced by several smart ways. Namely, the modification of supermolecular structure of semicrystalline polymers is particularly important. The morphology can be controlled by several methods, however, one of the most important and widely applied in the plastics industry is the application of nucleating agents. The heterogeneous nuclei influence crystallization kinetics, size of spherulites and, consequently, resulting properties. The nucleation of isotactic polypropylene (PP) is of particular interest due to its commercial importance and, consequently, intensive efforts are directed towards developing efficient nucleators and clarifiers for this polymer.Isotactic polypropylene is polymorphic polymer; it can crystallize into three phases: monoclinic -phase, trigonal -phase and orthorhombic -phase. Commonly, it crystallizes into -phase . However, specific -nucleating agents are often added into the material, primarily to improve the transparency, whilst the shortening of processing time and some improvement of mechanical properties are bonuses. For this purpose, powders of various compounds such as sodium benzoate, sorbitol derivatives and organophosphate salts have been developed.One of the often used -nucleating agent is 1,3:2,4-bis-(methylbenzylidene)sorbitol [2, 3]. Sorbitol-based
nucleating agents are soluble in concentration below 2 wt.% in molten PP at elevated temperatures . Upon cooling, the sorbitol-based compounds are capable of self-organizing in the polymer melt in the form of a three dimesional fibrillar network with characteristic dimensions in the nanometer range that causes the nucleation of PP, presumably due to epitaxial growth. The sorbitol derivatives improve optical properties with respect to clarity and haze dramatically. However, due to its sugar-based structure they has pure thermal stability during processing .The weathering of polymeric materials plays an important role for their service performance. The presence of tertiary carbon in the backbone of isotactic polypropylene is the reason of its high sensitivity to UV light, which is the most severe component of solar radiation. As generally accepted, degradation reactions of semicrystalline polymers proceed predominantly in the amorphous regions; nevertheless, morphology factors, such as the size, arrangement and distribution of the crystalline regions, play an important role in the degradation process as well. Thus, degradability of semicrystalline polymers is significantly influenced by their supermolecular structure. Many works deal with photodegradation of polypropylene [e.g. 6-10]. However, the effect of 1,3:2,4-bis-(methylbenzylidene)sorbitol nucleating agent on photodegradation of PP has not been complexly described yet. Thus, in this work, the pohotooxidation behaviour of PP containing several concentrations of this nucleating agent and neat PP is compared.
Latest Trends on Engineering Mechanics, Structures, Engineering Geology
ISSN: 1792-4294 424 ISBN: 978-960-474-203-5
2 Experimental2.1 Materials and SpecimensThe basic material used throughout this study was isotactic PP homopolymer Mosten GB 005 manufactured by Chemopetrol Litvnov a. s., the Czech Republic. The materials was characterized by a melt flow index of 5 g/10 min (2.16 kg, 230 C, ISO 1133), a weight average molecular weight of 360 000 (GPC) and an isotacticity index of 98 % (ISO 9113). The material was stabilised by a standard package based on phenol-phosphite stabilizers.The starting material GB 005 was modified by -nucleating agent Millad 3988 based on 1,3:2,4-di(3,4- dimethylbenzylidene) sorbitol. This nucleating agent was produced by Milliken Chemical. The concentrations applied were 0, 0.2, 0.5 and 0.8 wt. %. Blends were processed using twin-screw extruder Brabender DSK 42/6D and finally pelletized.Plates with dimensions of 125x60x0.2 mm were compression-moulded from all the materials. The material was put into preheated mould and after 5 min pressing at 210 C, the plates were cooled at 20 C.
2.2 UV-exposureRectangular specimens cut from the compression-moulded plates were irradiated at 50 C in Original Hanau XENOTEST 150. The exposure times varied from 0 to 528 h.
2.3 Infrared SpectroscopyA Nicolet Impact 400 spectrometer with nominal resolution of 2 cm-1 was employed in transmission mode with a 64-scan summation. Molecular degradation was characterized by carbonyl index AC/AR where AC is the area of the carbonyl absorption bands (in the range from 1 700 to 1 800 cm-1) and AR is the area of a reference band not affected by photooxidation and varying crystallinity (in the range from 2 700 to 2 750 cm-1) .
2.4 Differential Scanning CalorimetryA Perkin-Elmer Pyris 1 differential scanning calorimeter was used to observe melting, re-crystallization and re-melting of the specimens. Thermograms were recorded at a rate of 10 C/min under nitrogen purge (20 cm3/s). Approximately 4 mg of irradiated materials were heated to 220 C. Then the samples were held at 220 C for 5 min, cooled to 100 C and finally heated to 190 C.
2.5 Optical StereomicroscopyIn order to study surface of the degraded samples, a Zeiss Stemi 2000-C microscope was used. Micrographs of the observed surface were taken using a SONY F-717 digital camera.
3 Results and Discussion3.1 MeltingThe evolution of melting curves of neat and nucleated samples under study is presented in Figure 1. The exposure times of 0, 60, 120, 192, 336, 432, 480 and 528 hour are chosen as representatives. The interval of the melting is similar for all nucleated samples. Neat PP melts in slightly broader interval and also the shape of the peak is different as compared to nucleated samples; the peak is flat without distinct top. This points to formation of crystallites with narrower distribution of the size in heterogeneously nucleated materials. During the UV-irradiation the melting endotherms do not significantly change up to the 336 hours. However, at prolonged exposure time the interval of melting gradually shifts to lower temperatures in all cases. Moreover, the splitting of the peaks occurs. Finally, they are very flat with several maximums. The decrease of melting temperature of the materials upon the UV-irradiation is caused by erosion of the surfaces of the crystallites decreasing their thermodynamic stability .
Figure 1. Melting thermograms of UV-irradiated polypropylenes
Latest Trends on Engineering Mechanics, Structures, Engineering Geology
ISSN: 1792-4294 425 ISBN: 978-960-474-203-5
3.2 Evolution of Carbonyl By-ProductsThe evolution of the carbonyl index of all samples upon UV-irradiation is shown in Figure 2. Generally, two steps can be distinguished. First, an induction period occurs and second, after an induction period the slope of the curves dramatically increases. The results indicate that the degradation of all samples is not dramatically different. In initiative time of exposure (0-150 hours) carbonyl index values are zero and they are not marked in the graph. After this period carbonyl index begins slightly increase. After this induction period (approx, 250 hours of UV-exposure) carbonyl index rapidly increases. This rapid growth starts quite earlier in the case of neat PP and PP with 0.8 wt. % of nucleating agent. Final values of carbonyl index of these samples are consequently about one point higher than that of PP with o 0.2 and 0.5 wt. % of nucleating agent. Nevertheless, the difference in degradation kinetics of neat and variously nucleated samples is not significant and the presence of nucleating agent seems to not influence the process of carbonyl by-product formation during photooxidation.
Figure 2. Evolution of carbonyl index upon UV-irradiation
3.3 Surface CrackingUpon UV-irradiation the creation of surface cracking was observed. The cracks were not observed until 228 hours of irradiation. With prolonged exposure the c